Template:Infobox silicon Silicon (Template:PronEng or Template:IPA, Template:Lang-la) is the chemical element that has the symbol Si and atomic number 14. A tetravalent metalloid, silicon is less reactive than its chemical analog carbon. As the eighth most common element in the universe by mass, silicon occasionally occurs as the pure free element in nature, but is more widely distributed in dusts, planetoids and planets as various forms of silicon dioxide or silicate. On Earth, silicon is the second most abundant element (after oxygen) in the crust, making up 25.7% of the crust by mass.
Silicon has many industrial uses. Elemental silicon is the principal component of most semiconductor devices, most importantly integrated circuits or microchips. Silicon is widely used in semiconductors because it remains a semiconductor at higher temperatures than the semiconductor germanium and because its native oxide is easily grown in a furnace and forms a better semiconductor/dielectric interface than almost all other material combinations.
In the form of silica and silicates, silicon forms useful glasses, cements, and ceramics. It is also a component of silicones, a class-name for various synthetic plastic substances made of silicon, oxygen, carbon and hydrogen, often confused with silicon itself.
Silicon is an essential element in biology, although only tiny traces of it appear to be required by animals. It is much more important to the metabolism of plants, particularly many grasses, and silicic acid (a type of silica) forms the basis of the striking array of protective shells of the microscopic diatoms.
The outer electron orbitals (half filled subshell holding up to eight electrons) have the same structure as in carbon and the two elements are very similar chemically. Even though it is a relatively inert element, silicon still reacts with halogens and dilute alkalis, but most acids (except for some hyper-reactive combinations of nitric acid and hydrofluoric acid) do not affect it. Having four bonding electrons however gives it, like carbon, many opportunities to combine with other elements or compounds under the right circumstances.
Both silicon and carbon are semiconductors, readily either donating or sharing their four outer electrons allowing many different forms of chemical bonding. Pure silicon has a negative temperature coefficient of resistance, since the number of free charge carriers increases with temperature. The electrical resistance of single crystal silicon significantly changes under the application of mechanical stress due to the piezoresistive effect.
In its crystalline form, pure silicon has a gray color and a metallic luster. It is similar to glass in that it is rather strong, very brittle, and prone to chipping.
Measured by mass, silicon makes up 25.7% of the Earth's crust and is the second most abundant element on Earth, after oxygen. Pure silicon crystals are only occasionally found in nature; they can be found as inclusions with gold and in volcanic exhalations. Silicon is usually found in the form of silicon dioxide (also known as silica), and silicate.
Silica occurs in minerals consisting of (practically) pure silicon dioxide in different crystalline forms. Sand, amethyst, agate, quartz, rock crystal, chalcedony, flint, jasper, and opal are some of the forms in which silicon dioxide appears. (They are known as "lithogenic", as opposed to "biogenic", silicas.)
Silicon also occurs as silicates (various minerals containing silicon, oxygen and one or another metal), for example feldspar. These minerals occur in clay, sand and various types of rock such as granite and sandstone. Asbestos, feldspar, clay, hornblende, and mica are a few of the many silicate minerals.
See also Category:Silicate minerals
Silicon has numerous known isotopes, with mass numbers ranging from 22 to 44. 28Si (the most abundant isotope, at 92.23%), 29Si (4.67%), and 30Si (3.1%) are stable; 32Si is a radioactive isotope produced by argon decay. Its half-life has been determined to be approximately 170 years (0.21 MeV), and it decays by beta - emission to 32P (which has a 14.28 day half-life ) and then to 32S.
Template:Expand-section For examples of silicon compounds see silicate, silane (SiH4), silicic acid (H4SiO4), silicon carbide (SiC), silicon dioxide (SiO2), silicon tetrachloride (SiCl4), silicon tetrafluoride (SiF4), and trichlorosilane (HSiCl3).
See also Category:Silicon compounds
As the second most abundant element in the earth's crust, silicon is vital to the construction industry as a principal constituent of natural stone, glass, concrete and cement. Silicon's greatest impact on the modern world's economy and lifestyle has resulted from its use as the substrate in the manufacture of discrete electronic devices such as power transistors, and in the development of integrated circuits such as computer chips.
- The largest application of pure silicon (metallurgical grade silicon) is in aluminium-silicon alloys, often called "light alloys", to produce cast parts, mainly for automotive industry. (This represents about 55% of the world consumption of pure silicon.)
- Steel and cast iron: Silicon is an important constituent of some steels, and it is used in the production process of cast iron. It is introduced as ferrosilicon or silicocalcium alloys.
In electronic applications
- Pure silicon is also used to produce ultra-pure silicon for electronic and photovoltaic applications:
- Semiconductor: Ultrapure silicon can be doped with other elements to adjust its electrical response by controlling the number and charge (positive or negative) of current carriers. Such control is necessary for transistors, solar cells, microprocessors, semiconductor detectors and other semiconductor devices which are used in electronics and other high-tech applications.
- Photonics: Silicon can be used as a continuous wave Raman laser to produce coherent light. (Though it is ineffective as a light source.)
- LCDs and solar cells: Hydrogenated amorphous silicon is widely used in the production of low-cost, large-area electronics in applications such as LCDs. It has also shown promise for large-area, low-cost thin-film solar cells.
The second largest application of silicon (about 40% of world consumption) is as a raw material in the production of silicones, compounds containing silicon-oxygen and silicon-carbon bonds that have the capability to acting as bonding intermediates between glass and organic compounds, and to form polymers with useful properties such as impermeability to water, flexibility and resistance to chemical attack. Silicones are used in waterproofing treatments, moulding compounds and mould-release agents, mechanical seals, high temperature greases and waxes, caulking compounds and even in applications as diverse as breast implants and explosives and pyrotechnics  .
- Construction: Silicon dioxide or silica in the form of sand and clay is an important ingredient of concrete and brick and is also used to produce Portland cement.
- Pottery/Enamel is a refractory material used in high-temperature material production and its silicates are used in making enamels and pottery.
- Glass: Silica from sand is a principal component of glass. Glass can be made into a great variety of shapes and with many different physical properties. Silica is used as a base material to make window glass, containers, insulators, and many other useful objects.
- Abrasives: Silicon carbide is one of the most important abrasives.
- Silly Putty was originally made by adding boric acid to silicone oil. Now name-brand Silly Putty also contains significant amounts of elemental silicon. (Silicon binds to the silicone and allows the material to bounce 20% higher.)
See also Category:Silicon compounds
Silicon is commercially prepared by the reaction of high-purity silica with wood, charcoal, and coal, in an electric arc furnace using carbon electrodes. At temperatures over 1900 °C, the carbon reduces the silica to silicon according to the chemical equation
- SiO2 + C → Si + CO2.
- SiO2 + 2C → Si + 2CO.
Liquid silicon collects in the bottom of the furnace, and is then drained and cooled. The silicon produced via this process is called metallurgical grade silicon and is at least 98% pure. Using this method, silicon carbide, SiC, can form. However, provided the amount of SiO2 is kept high, silicon carbide may be eliminated, as explained by this equation:
- 2 SiC + SiO2 → 3 Si + 2 CO.
The use of silicon in semiconductor devices demands a much greater purity than afforded by metallurgical grade silicon. Historically, a number of methods have been used to produce high-purity silicon.
Early silicon purification techniques were based on the fact that if silicon is melted and re-solidified, the last parts of the mass to solidify contain most of the impurities. The earliest method of silicon purification, first described in 1919 and used on a limited basis to make radar components during World War II, involved crushing metallurgical grade silicon and then partially dissolving the silicon powder in an acid. When crushed, the silicon cracked so that the weaker impurity-rich regions were on the outside of the resulting grains of silicon. As a result, the impurity-rich silicon was the first to be dissolved when treated with acid, leaving behind a more pure product.
In zone melting, also called zone refining, the first silicon purification method to be widely used industrially, rods of metallurgical grade silicon are heated to melt at one end. Then, the heater is slowly moved down the length of the rod, keeping a small length of the rod molten as the silicon cools and re-solidifies behind it. Since most impurities tend to remain in the molten region rather than re-solidify, when the process is complete, most of the impurities in the rod will have been moved into the end that was the last to be melted. This end is then cut off and discarded, and the process repeated if a still higher purity is desired.
Today, silicon is purified by converting it to a silicon compound that can be more easily purified than in its original state, and then converting that silicon element back into pure silicon. Trichlorosilane is the silicon compound most commonly used as the intermediate, although silicon tetrachloride and silane are also used. When these gases are blown over silicon at high temperature, they decompose to high-purity silicon.
- SiCl4 + 2 Zn → Si + 2 ZnCl2.
However, this technique was plagued with practical problems (such as the zinc chloride byproduct solidifying and clogging lines) and was eventually abandoned in favor of the Siemens process.
In the Siemens process, high-purity silicon rods are exposed to trichlorosilane at 1150 °C. The trichlorosilane gas decomposes and deposits additional silicon onto the rods, enlarging them according to chemical reactions like
- 2 HSiCl3 → Si + 2 HCl + SiCl4.
Silicon produced from this and similar processes is called polycrystalline silicon. Polycrystalline silicon typically has impurity levels of less than 10−9.
- 3SiCl4 + Si + 2H2 → 4HSiCl3
- 4HSiCl3 → 3SiCl4 + SiH4
- SiH4 → Si + 2H2
The majority of silicon crystals grown for device production are produced by the Czochralski process, (CZ-Si) since it is the cheapest method available and it is capable of producing large size crystals. However, silicon single-crystals grown by the Czochralski method contain impurities since the crucible which contains the melt dissolves. For certain electronic devices, particularly those required for high power applications, silicon grown by the Czochralski method is not pure enough. For these applications, float-zone silicon (FZ-Si) can be used instead. It is worth mentioning though, in contrast with CZ-Si method in which the seed is dipped into the silicon melt and the growing crystal is pulled upward, the thin seed crystal in the FZ-Si method sustains the growing crystal as well as the polysilicon rod from the bottom. As a result, it is difficult to grow large size crystals using the float-zone method. Today, all the dislocation-free silicon crystals used in semiconductor industry with diameter 300mm or larger are grown by the Czochralski method with purity level significantly improved.
Different forms of silicon
Broken silicon ingot
This article needs additional citations for verification. (August 2006) (Learn how and when to remove this template message)
This article possibly contains original research. (December 2007) (Learn how and when to remove this template message)
Since silicon is similar to carbon, particularly in its valency, some people have proposed the possibility of silicon-based life. One main detraction for silicon-based life is that unlike carbon, silicon does not have the tendency to form double and triple bonds.
Although there are no known forms of life that rely entirely on silicon-based chemistry, there are some that rely on silicon minerals for specific functions. Some bacteria and other forms of life, such as the protozoa radiolaria, have silicon dioxide skeletons, and the sea urchin has spines made of silicon dioxide. These forms of silicon dioxide are known as biogenic silica. Silicate bacteria use silicates in their metabolism.
Life as we know it could not have developed based on a silicon biochemistry. The main reason for this fact is that life on Earth depends on the carbon cycle: autotrophic entities use carbon dioxide to synthesize organic compounds with carbon, which is then used as food by heterotrophic entities, which produce energy and carbon dioxide from these compounds. If carbon was to be replaced with silicon, there would be a need for a silicon cycle. However, silicon dioxide precipitates in aqueous systems, and cannot be transported among living beings by common biological means.
As such, another solvent would be necessary to sustain silicon-based life forms; it would be difficult (if not impossible) to find another common compound with the unusual properties of water which make it an ideal solvent for carbon-based life. Larger silicon compounds analogous to common hydrocarbon chains (silanes) are also generally unstable owing to the larger atomic radius of silicon and the correspondingly weaker silicon-silicon bond; silanes decompose readily and often violently in the presence of oxygen making them unsuitable for an oxidizing atmosphere such as our own. Silicon also does not readily participate in pi-bonding (the second and third bonds in triple bonds and double bonds are pi-bonds) as its p-orbital electrons experience greater shielding and are less able to take on the necessary geometry. Furthermore, although some silicon rings (cyclosilanes) analogous to common the cycloalkanes formed by carbon have been synthesized, these are largely unknown. Their synthesis suffers from the difficulties inherent in producing any silane compound, whereas carbon will readily form five-, six-, and seven-membered rings by a variety of pathways (the Diels-Alder reaction is one naturally-occurring example), even in the presence of oxygen. Silicon's inability to readily form long silane chains, multiple bonds, and rings severely limits the diversity of compounds that can be synthesized from it. Under known conditions, silicon chemistry simply cannot begin to approach the diversity of organic chemistry, a crucial factor in carbon's role in biology.
However, silicon-based life could be construed as being life which exists under a computational substrate. This concept is yet to be explored in mainstream technology but receives ample coverage by sci-fi authors.
A. G. Cairns-Smith has proposed that the first living organisms to exist were forms of clay minerals—which were probably based around the silicon atom.
Silicon was first identified by Antoine Lavoisier in 1787 (as a component of the Latin Template:Wdy, or silicis (meaning what were more generally termed "the flints" or "Hard Rocks" during the Early Modern era where nowadays as we would say "silica" or "silicates"), and was later mistaken by Humphry Davy in 1800 for a compound. In 1811 Gay-Lussac and Thénard probably prepared impure amorphous silicon through the heating of potassium with silicon tetrafluoride. It was first discovered as an element by Berzelius in 1823. In 1824, Berzelius prepared amorphous silicon using approximately the same method as Lussac. Berzelius also purified the product by repeatedly washing it.
- Los Alamos National Laboratory: Silicon
- Elastic Waves in Solids II, Eugène Dieulesaint, Daniel Royer (Springer) 2000 (ISBN 3-540-65931-5) (speed of sound)
|Wikimedia Commons has media related to Silicon.|
|File:Wiktionary-logo-en-v2.svg||Look up silicon in Wiktionary, the free dictionary.|
Template:Link FA af:Silikon ar:سليكون ast:Siliciu be:Крэмній bs:Silicijum bg:Силиций ca:Silici cs:Křemík co:Siliciu cy:Silicon da:Silicium de:Silicium et:Räni el:Πυρίτιο eo:Silicio eu:Silizio fur:Silici ga:Sileacan gl:Silicio (elemento) gu:સિલિકોન ko:규소 hy:Սիլիցիում hi:सिलिकन hr:Silicij io:Siliko id:Silikon is:Kísill it:Silicio he:צורן ht:Silisyòm la:Silicium lv:Silīcijs lb:Silizium lt:Silicis jbo:cancmu hu:Szilícium mk:Силициум ml:സിലിക്കണ് mi:Takawai mr:सिलिकॉन ms:Silikon mn:Цахиур nah:Tecpatli nl:Silicium no:Silisium nn:Silisium oc:Silici uz:Kremniy nds:Silizium qu:Ullayayaq scn:Siliciu simple:Silicon sk:Kremík sl:Silicij sr:Силицијум sh:Silicij fi:Pii (alkuaine) sv:Kisel ta:சிலிக்கான் th:ซิลิคอน tg:Силитсий uk:Кремній zh-yue:矽 Template:WikiDoc Sources